## Analysis of Sensitivity for Low-Pass Multilayer

## Optical Filters

*A.Massaro, L.Pierantoni, Member IEEE, C.Ciandrini, T.Rozzi, *

*Fellow IEEE*

Dipartimento di Elettromagnetismo e Bioingegneria, Università Politecnica delle Marche, via Brecce Bianche
12,I-60131, Ancona, Italy. e-mail: [email protected], [email protected], [email protected]**.**

**Abstract — Integrated optical and millimetric circuits **

**produced by standard thin film-based technology suffer **
**from manufacturing imperfections resulting in degradation **
**of the absorption/diffraction response. Deposition through **
**rf-bias sputtering is of particular interest in order to design **
**an optical multilayered (Si and SiO2) filter. Geometrical **

**imperfections like roughness at layer boundaries however **
**gradually increase with the number of deposited layers. The **
**low-pass filter specifications present high sensitivity to the **
**errors of the exact values of ideal thickness and of ideal **
**refractive indices. In this contribution, we evaluate the **
**sensitivity of the specifications with respect to deviation **
**from the exact values of refractive indices and thicknesses. **

I. INTRODUCTION

In optical filtering applications it is very important to determine the exact fabrication conditions.We analyze a low-pass filter multilayered structure presenting both i) a high refractive index nH; ii) a low refractive index nL (see

Fig.2) as reported in [1]-[3]. Due to deviations in the fabrication process (deposition technique, Fig.1), the frequency characteristics can be significantly affected. It possible to reduce the amplitude of roughness below 0.3 nm through the use of rf-bias sputtering[1], but for a high number of layers the last few layers may present problems, whereas it is known that low-pass multilayered (Si and SiO2) filters are very sensitive to the parameters

of the layers (refractive index and layer thickness). The goal of the present contribution is the analysis of the actual response of a multilayer (see Fig.2) filter originally designed from a Chebyshev prototype polynomials in order to fullfill low-pass specifications (Fig.3); for simplicity of analysis, we assume that all the refractive indices are non-absorbing and that the electrical length și

are equal. After this prototype analysis, we perform a 3D full-wave simulation by using the Transmission Line Matrix-Integral Equation (TLMIE) method [5-6], where we vary the refractive index and estimate the Q factor sensitivity.

II. THEORY

The low-pass filter of Fig. 2 was designed according to Chebyshev prototype in order to yield the squared magnitude response of the form

2
2 2
1
( )
1 *N*( \ *c*)
*H j*
*h T*
Z
Z Z
(1)

where TN(x) is the Nth-order (number of layers)

Chebyshev (Fig. 3) polynomial defined by

1 1

( ) cos( cos ( ) cosh( cosh ( ))

*N*

*T* *x* *N* *x* *N* *x* _{ (2)}

Ȧc is the cutoff angular frequency. The filter

specifications for the magnitude response in the passband and in the stopband are respectively:

1

1t *H j*( Z t 1 G Z dZ*c* (3)
*H j*(

### Z

) d### G

_{2 }

### Z

t### Z

*(4) The Chebyshev polynomials (2) can be generated recursively by:*

_{r} *T _{N}*

_{}

_{1}( ) 2

*x*

*xT x*( )

_{N}*T*

_{N}_{}

_{1}( )

*x*

(5) Since TN(x)=1 for any N, the squared magnitude response

at cutoff equals 1/(1+h2_{), and h}2_{ is thus determined from }

the passband ripple į1 as

2
2
2
1
1
1
(1 )
*sub*
*H*
*sub* *L*
*sub*
*H*
*sub* *L*
*n*
*n*
*n* *n*
*h*
*n*
*n*
*n* *n*
G
_{}
(6)

where the ripple factor has been established [4] for the ideally terminated multilayer. The required value of N for given stopband specifications is obtained from (1)-(4) as:

1 _{1}
2
2
2 2
2
1
cosh cosh *r*
*c*
*N*
*h*
G Z
G Z
_{}
§ § ·· § § ··
¨ ¨_{¨} ¸_{¸}¸ ¨ ¨ ¸¸
¨ _{©} _{¹}¸ _{©} _{©} _{¹}_{¹}
© ¹
(7)

We observe that the number of the layers depends on the exact values of the refractive indices of the multilayer, so it is very important for the sputtering system to define the exact deposition condition[1] (oxygen-flow rate, temperature of substrate, total gas flow-rate, total gas pressure). In Fig.6 we show the variation of N: (a) for a substrate with a refractive index near the value of Si, (b) for a layer with a refractive index near the value nL(SiO2).

In the sensitivity of the number of layers we assume equal optical lengths: nHtH=nLtL, where tH is the thickness

of the layer with a high refractive index, and tL the

thickness of the layer with a low refractive index. In Fig.5 we report the variation of the order N with tLby

varying the thickness of tH of 1nm and 0.4 nm, in

accordance with the roughness of the rf-sputtering technique. By fixing tLmore layers are necessary in order

to satisfy the same specifications, in the case of variation of the thickness tH. Hence, , it is now possible first i) to

evaluate the number of layers N, for a given specification, and then ii) the exact number N considering the roughness error. In Fig.7 we report the shift of the Chebyshev poles for a variation of tH of 1 nm; it is seen

that when the thickness tHincreases up to 226 nm, the

minimum number of layers that can satisfy the specifications increases from N=7 to N=8.

It is also possible to analyze the effect of the sensitivity by utilizing the ray model[5]: For a multilayer of homogeneous layers of alternately low and high refractive indices n3 and n2 and of thickness h3 and h2,

placed between two homogeneous media of refractive indices n0 and nsub, if we assume P=1 and set (TE

analysis)
2
2 _{cos}
*H* *H* *H*
*n d*
S
E T
O , 3
2 _{cos}
*L* *L* *L*
*n d*
S
E T
O
,*p _{H}*

*n*cosT

_{H}

_{H},*p _{L}*

*n*cos , T

_{L}

_{L}*p*

_{sub o}_{,}H

_{sub o}_{,}/PcosT

_{sub o}_{,}(8) where ș is the ray-angle in the dielectric layers.

The characteristic matrix of one period (t=dh+dL) is

2

2 3 2 3 2 3 2 3

2 3 2 3 2 3 2 3

cos cos sin sin cos sin sin cos

.

sin cos cos sin cos cos sin sin

*L*
*H* *L* *H*
*H*
*H* *L*
*L*
*M t*
*p* *i* *i*
*p* *p* *p*
*p*
*ip* *ip*
*p*
E E E E E E E E
E E E E E E E E
ª _{} _{} _{} º
« »
« »
« »
« »
¬ ¼
(9)
For 2N films we have

11 12 2 21 22

### ( )

*N*

*M*

*M*

*M*

*Nt*

*M*

*M*

### ª

### º

### «

### »

### ¬

### ¼

(10) where11 cos 2cos 3 *L* sin 2sin 3 *N* 1( ) *N* 2( )
*H*
*p*
*M* *u* *a* *u* *a*
*p*
E E E E
§ ·
¨ ¸
© ¹
12 2 3 2 3 1
1 1

cos cos sin cos *N* ( )

*L* *H*
*M* *i* *u* *a*
*p* E E *p* E E
§ ·
_{¨} _{¸}
© ¹

21 *H*sin 2cos 3 *L*cos 2sin 3 *N*1( )
*M* *i p* E E *p* E E *u* *a*
22 cos 2cos 3 *H*sin 2sin 3 *N* 1( ) *N* 2( )

*L*
*p*
*M* *u* *a* *u* *a*
*p*
E E E E
§ ·
¨ ¸
© ¹
2 3 2 3
1

cos cos sin sin

2
*H* *L*
*L* *H*
*p* *p*
*a*
*p* *p*
E E §_{¨} ·_{¸} E E
© ¹
(11)
*where UN*(x) are the Chebyshev Polynomials of the

second kind. We observe that for the general case the reflectivity and the transmissivity are given by [5]

2
2 11 12 21 22
11 12 21 22
( ) ( )
( ) ( )
*sub*
*sub* *sub*
*sub* *o*
*o*
*M* *M p* *p* *M* *M p*
*r*
*M* *M p* *p* *M* *M p*
(12)
2
11 12 21 22
2
( ) ( )
*sub* *sub*
*sub* *o*
*o* *o*
*p* *p*
*p* *M* *M p* *p* *M* *M p*
(13)
In Fig.8,9,10 is shown the sensitivity of the reflectivity
for different values of refractive indices and thicknesses
(normal incidence, no=nsub=1).

III. TLMIERESULTS

*In the TLMIE method the physical structure is enclosed *
in a imaginary (rectangular) “box”, whose sides are the
boundaries for the TLM-region (inside) and for the
homogeneous regions (free-space/bulk region), [7]. This
naturally leads to define the cavity-domain for the
calculation of the Q-factor as the aforementioned “box”.
We have:
0
*L*
*U*
*Q*
*W*
Z _{ (14) }

where Ȧ0 is the work angular frequency, U is the energy

stored in the multilayered structure integrated on a period, and WL is the dissipated power given by

Poynting vector Py(x,y,z;t)=EzHx-ExHz.

We observe that the Poynting vector is taken by starting from a reference plane (Fig.4), and in this case, in order to evaluate the Q factor for each frequency, we use a sinusoidal excitations of angular frequency Ȧ0. The

stored energy is evaluated by integrating the density (E2

x+E2z) in the period of excitation and by using the

Boundary Oriented Field-Mapping (BOFM) [6] approach. In Fig.11 we report the variation of Q factor and power losses in the case of a seven (Si and SiO2)

layer low-pass filter; it is clear that in the transition band (middle region) the Q factor shows high sensitivity with respect to the refractive index (as shown in Fig.6).

IV. CONCLUSION

In this contribution we deal with a real problems widely present in the realization of thin film layer optical filters: i) the effect of roughness at layer boundaries, ii) deviations from the exact values of the refractive indices and thickness, showing how these affect the realization of optical (Si and SiO2) filters. By using the accurate

full-wave TLMIE method we investigate the behaviour Q factor as a function of optical parameters.

Fig. 1. Cross-sectional photographs in the vicinity of (a) the substrate and (b) the top surface.

Fig. 2. Schematic representation of a low-pass multilayer filter with roughness of amplitude ǻ and n0=1(air).

Fig.3. Classical low-pass filter specifications for the magnitude response and Type-I Chebyshev magnitude response of order N.

Fig.4. TLMIE simulated optical low pass filter.

Fig.5. Variation of number of layers with the thickness tLfor

ȜC=1.55 µm, Ȝr=0.09 µm, nsub=3.3, nL =1.45, į2=0.15 (N1 for

th=240 nm, N2 for th=230 nm, and N3 for th=239.6 nm).

Fig.6. Variation of number of layers N1=N with nsub (a) using

ȜC=1.55 µm, Ȝr=0.08 µm, nH=3.24, nL=1.45, į2=0.20, with nL

(b) using ȜC=1.55 µm, Ȝr=0.009 µm, nH=3.45, nsub =1.45, į2

=0.15.

Fig.7: Variation of position of Chebyshev poles for a multilayer of 7 layers (sufficient to satisfy the specifications). A is the

vector of poles for thickness tL=100nm, th=225nm ȜC=1.565

µm, Ȝr=0.09 µm, nsub=3, nH=3.24, nL=1.44, į2=0.15, į1=0.047;

B is the pole vector related to a variation of tH of 1nm(tH=226

nm).

Fig.8. Reflectivity using four Si/SiO2 layers with nH=3.45,

tH=0.4 µm, tL=0.26 µm (R for nL=2, R1 for nL=1.46, and R2 for

nL=2.2).

Fig.9. Reflectivity using four Si/SiO2 layers with nH=3.45, nL=2,

tH=0.4 µm, (R for tL=0. 260 µm, R1 for tL=0.266 µm, and R2

for tL=0.27 µm).

Fig.10. Reflectivity using four Si/SiO2 layers with, tL=0.26 µm,

tH=0.4 µm, nL=2 (R for nH=3.45, R1 for nH=3.50, and R2 for

nH=3.40).

Fig.11. TLMIE method- Q factor (above) and normalized power lost (below) of a simulated low-pass optical

multilayered (7 layers) filter. a) tL=100nm, th=225nm, ,

nsub=3, nH=3.24, nL =1.4,b) tL=100nm, th=225nm, nsub=3,

nH=3.24, nL =1.44, c) tL=100nm, th=225nm, , nsub=3,5,

nH=3.34, nL=1.5.

REFERENCES

[1] T. Sato, T. Sasaki, K.Tsuchida, K.Shiraishi, S. Kawakami,
“Scattering mechanism and reduction of insertion losses in
*a laminated polarization splitter”, Applied Optics, Vol. 33 *
pp. 6925-6934, October 1994

[2] Rhong-Chung Tyan ,Pang_Chen Sun, Axel Scherer, and
Yesha Yahu Fainman, “Polarizing beam splitter based on
the anisotropic spectral reflectivity characteristic of
* form-birefringent multilayer gratings”, Optics Letters vol.21,*
no.10/May 15 pp. 761-763.

[3] A. Massaro, A. Di Donato, T.Rozzi, “Negative uniaxial
optical behaviour of laminated polarization
*beam-splitters” GaAs2002 Conference, Milan, pp.133. *

[4] T.C. Chen, “Optimised design of odd-order optical
lowpass and highpass multilayer filters by method of
*coefficient matching”, IEE Proceedings, Vol.135,No.2, *
April 1988.

*[5] M. Born and E. Wolf, Principles of Optics, 6th ed., Ed.: *
Cambridge University Press, 1980.

[6] J. Rebel, “On the foundations of the Transmission Line
*Matrix Method”, Ph.D Thesis, Technische Univ. *

*Muenchen. December1999. *

[7] L. Pierantoni, S. Lindenmeier and P. Russer, “A Combination of Integral Equation Method and FD/TLM

*Method for Efficient Solution of EMC Problems”, 27th*

*European Microwave Conf. (EuMC), Jerusalem, Israel, *

8-12 September, 1997, pp. 93